14:635:407:02 Homework III Solutions


 Magdalen Morton
 2 years ago
 Views:
Transcription
1 14:635:407:0 Homework III Solutions 4.1 Calculate the fraction of atom sites that are vacant for lead at its melting temperature of 37 C (600 K). Assume an energy for vacancy formation of 0.55 ev/atom. In order to compute the fraction of atom sites that are vacant in lead at 600 K, we must employ Equation 4.1. As stated in the problem, Q v = 0.55 ev/atom. Thus, N v N = exp Q v = exp kt 0.55 ev / atom ( ev /atom K) (600 K) = Calculate the number of vacancies per cubic meter in iron at 850C. The energy for vacancy formation is 1.08 ev/atom. Furthermore, the density and atomic weight for Fe are 7.65 g/cm 3 and g/mol, respectively. Determination of the number of vacancies per cubic meter in iron at 850C (113 K) requires the utilization of Equations 4.1 and 4. as follows: N v = N exp Q v = N A Fe kt A Fe exp Q v kt And incorporation of values of the parameters provided in the problem statement into the above equation leads to N v = ( atoms /mol)(7.65 g /cm 3 ) g /mol exp 1.08 ev/ atom ( ev /atom K) (850C + 73 K) = cm 3 = m 3
2 4.5 For both FCC and BCC crystal structures, there are two different types of interstitial sites. In each case, one site is larger than the other, and is normally occupied by impurity atoms. For FCC, this larger one is located at the center of each edge of the unit cell; it is termedd an octahedral interstitial site. On the other hand, with BCC the larger site type is found at positions that is, lying on {100} faces, and situated midway between two unit cell edges on this face and onequarter of the distance between the other two unit cell edges; it is termed a tetrahedral interstitial site. For both FCC and BCCC crystal structures, compute the radius r of an impurity atom that will just fit into one of these sites in terms of the atomic radius R of the host atom. In the drawing below is shown the atoms on the (100) facee of an FCC unit cell; the interstitial site is at the center of the edge. The diameter of an atom that will just fit into this site (r) is just thee difference between that unit cell edge length (a) and the radii of the two host atoms that are located on either side of the site (R); that is r = a R However, for FCC a is related to R according to Equation 3.1 as a R ; therefore, solving for r from the above equation gives r = a R = R R = 0.41R
3 A (100) face of a BCC unit cell is shown below. The interstitial atom thatt just fits into this t interstitial site is shown by the small circle. It is situated in the plane of this (100) face, midway between the two vertical unitt cell edges, and one quarter of the distance between the bottom and top cell edges. From the right triangle that is defined by the three arrows we may write a + a 4 = (R r) However, from Equation 3.3, a = 4R R, and, therefor re, making thiss substitution, the above equation takes the form 3 4R 3 + 4R4 4 3 = R + Rr + r After rearrangement the following f quadratic equation results: r + Rr 0.667R = 0 And upon solving for r:
4 r (R) (R) (4)(1)(0.667R ) R.58R And, finally R.58R r() 0.91R R.58R r().91r Of course, only the r(+) root is possible, and, therefore, r = 0.91R. Thus, for a host atom of radius R, the size of an interstitial site for FCC is approximately 1.4 times that for BCC.
5 4.15 The concentration of carbon in an ironcarbon alloy is 0.15 wt%. What is the concentration in kilograms of carbon per cubic meter of alloy? In order to compute the concentration in kg/m 3 of C in a 0.15 wt% C wt% Fe alloy we must employ Equation 4.9 as C C " = C C C C C C Fe Fe 10 3 From inside the front cover, densities for carbon and iron are.5 and 7.87 g/cm 3, respectively; and, therefore C C " = g/cm g/cm = 11.8 kg/m Determine the approximate density of a highleaded brass that has a composition of 64.5 wt% Cu, 33.5 wt% Zn, and.0 wt% Pb. In order to solve this problem, Equation 4.10a is modified to take the following form: ave = C Cu Cu 100 C Zn Zn C Pb Pb And, using the density values for Cu, Zn, and Pb i.e., 8.94 g/cm 3, 7.13 g/cm 3, and g/cm 3 (as taken from inside the front cover of the text), the density is computed as follows: ave = wt% 8.94 g /cm wt% 7.13 g /cm 3.0 wt% g /cm 3 = 8.7 g/cm 3
6 4.18 Some hypothetical alloy is composed of 1.5 wt% of metal A and 87.5 wt% of metal B. If the densities of metals A and B are 4.7 and 6.35 g/cm 3, respectively, whereas their respective atomic weights are 61.4 and 15.7 g/mol, determine whether the crystal structure for this alloy is simple cubic, facecentered cubic, or bodycentered cubic. Assume a unit cell edge length of nm. In order to solve this problem it is necessary to employ Equation 3.5; in this expression density and atomic weight will be averages for the alloy that is ave = na ave V C N A Inasmuch as for each of the possible crystal structures, the unit cell is cubic, then V C = a 3, or ave = na ave a 3 N A And, in order to determine the crystal structure it is necessary to solve for n, the number of atoms per unit cell. For n =1, the crystal structure is simple cubic, whereas for n values of and 4, the crystal structure will be either BCC or FCC, respectively. When we solve the above expression for n the result is as follows: n = ave a3 N A A ave Expressions for A ave and ave are found in Equations 4.11a and 4.10a, respectively, which, when incorporated into the above expression yields n = 100 C A C a B 3 N A A B 100 C A C B A A A B
7 Substitution of the concentration values (i.e., C A = 1.5 wt% and C B = 87.5 wt%) as well as values for the other parameters given in the problem statement, into the above equation gives n = 100 ( wt% 4.7 g/cm wt% 8 nm) 3 ( atoms/mol) 6.35 g/cm wt% 61.4 g/mol 87.5 wt% 15.7 g/mol =.00 atoms/unit cell Therefore, on the basis of this value, the crystal structure is bodycentered cubic. 4.0 Gold forms a substitutional solid solution with silver. Compute the number of gold atoms per cubic centimeter for a silvergold alloy that contains 10 wt% Au and 90 wt% Ag. The densities of pure gold and silver are 19.3 and g/cm 3, respectively. To solve this problem, employment of Equation 4.18 is necessary, using the following values: C 1 = C Au = 10 wt% 1 = Au = 19.3 g/cm 3 = Ag = g/cm 3 A 1 = A Au = g/mol Thus N Au = C Au A Au Au N A C Au A Au Ag (100 C Au ) = ( atoms /mol) (10 wt%) (10 wt%)( g /mol) g /mol 19.3 g /cm 3 ( wt%) g /cm3 = atoms/cm 3
8 4.6 Cite the relative Burgers vector dislocation line orientations for edge, screw, and mixed dislocations. The Burgers vector and dislocation line are perpendicular for edge dislocations, parallel for screw dislocations, and neither perpendicular nor parallel for mixed dislocations. 4.7 For an FCC single crystal, would you expect the surface energy for a (100) plane to be greater or less than that for a (111) plane? Why? (Note: You may want to consult the solution to Problem 3.54 at the end of Chapter 3.) The surface energy for a crystallographic plane will depend on its packing density [i.e., the planar density (Section 3.11)] that is, the higher the packing density, the greater the number of nearestneighbor atoms, and the more atomic bonds in that plane that are satisfied, and, consequently, the lower the surface energy. From the 1 solution to Problem 3.54, planar densities for FCC (100) and (111) planes are 4R and 1 R 3, respectively that is and R R (where R is the atomic radius). Thus, since the planar density for (111) is greater, it will have the lower surface energy. 4.8 For a BCC single crystal, would you expect the surface energy for a (100) plane to be greater or less than that for a (110) plane? Why? (Note: You may want to consult the solution to Problem 3.55 at the end of Chapter 3.) The surface energy for a crystallographic plane will depend on its packing density [i.e., the planar density (Section 3.11)] that is, the higher the packing density, the greater the number of nearestneighbor atoms, and the more atomic bonds in that plane that are satisfied, and, consequently, the lower the surface energy. From the 3 solution to Problem 3.55, the planar densities for BCC (100) and (110) are 16R and 3 8R, respectively that is and. Thus, since the planar density for (110) is greater, it will have the lower surface energy. R R
9 4.9 (a) For a given material, would you expect the surface energy to be greater than, the same as, or less than the grain boundary energy? Why? (b) The grain boundary energy of a smallangle grainn boundary iss less than for a highangle one. Why is this so? (a) The surface energy will be greater than the grain boundary energy. For grain boundaries, some atoms on one side of a boundary will bond to atoms on the other side; such is not the case for surface atoms. Therefore, there will be fewer unsatisfied bonds along a grain boundary. (b) The smallangle grain boundary energy is lower thann for a highangle one because more atoms bond across the boundary for the smallangle, and, thus, there are fewer unsatisfied bonds (a) Briefly describe a twin and a twin boundary. (b) Cite the difference between mechanical and annealing twins. (a) A twin boundary is an interface such that atoms on one side are located at mirror image positions of those atoms situated on the other boundary side. The region on one side of this boundary is called a twin. (b) Mechanical twins are produced as a result of mechanical deformation and generally occur in BCC and HCP metals. Annealing twins form during annealing heat treatments, most often in FCC metals For each of the following stacking sequences found in FCC metals, cite the type of planar defect that exists: (a)... A B C A B C B A C B A... (b)... A B C A B C B C A B C... Now, copy the stacking sequences and indicate the position(s) off planar defect(s) with a vertical dashed line. (a) The interfacial defect that exists for this stacking sequence iss a twin boundary, which occurs at the indicated position. The stacking sequence on one side of this position is mirrored on thee other side. (b) The interfacial defect that exists within this FCC stacking sequencee is a stacking fault, which occurs between the two lines. Within this region, the stacking sequence is HCP.
10 14:440:407 Section 0 Fall 010 SOLUTION OF HOMEWORK 04 Question 5.3: (a) Compare interstitial and vacancy atomic mechanisms for diffusion. (b) Cite two reasons why interstitial diffusion is normally more rapid than vacancy diffusion. Solution of 5.3: (a) With vacancy diffusion, atomic motion is from one lattice site to an adjacent vacancy. Selfdiffusion and the diffusion of substitutional impurities proceed via this mechanism. On the other hand, atomic motion is from interstitial site to adjacent interstitial site for the interstitial diffusion mechanism. (b) Interstitial diffusion is normally more rapid than vacancy diffusion because: (1) interstitial atoms, being smaller, are more mobile; and () the probability of an empty adjacent interstitial site is greater than for a vacancy adjacent to a host (or substitutional impurity) atom. Question 5.4: Briefly explain the concept of steady state as it applies to diffusion. Solution of 5.4: Steadystate diffusion is the situation wherein the rate of diffusion into a given system is just equal to the rate of diffusion out, such that there is no net accumulation or depletion of diffusing speciesi.e., the diffusion flux is independent of time. Question 5.6: The purification of hydrogen gas by diffusion through a palladium sheet was discussed in Section 5.3. Compute the number of kilograms of hydrogen that pass per hour through a 5mmthick sheet of palladium having an area of 0.0 m at 500C. Assume a diffusion coefficient of m /s, that the concentrations at the highand lowpressure sides of the plate are.4 and 0.6 kg of hydrogen per cubic meter of palladium, and that steadystate conditions have been attained. Solution of 5.6: This problem calls for the mass of hydrogen, per hour, that diffuses through a Pd sheet. It first becomes necessary to employ both Equations 5.1a and 5.3. Combining these expressions and solving for the mass yields M = JAt = DAt C x = ( m /s)(0.0 m kg /m3 ) (3600 s/h) m = kg/h
11 Question 5.8: A sheet of BCC iron 1 mm thick was exposed to a carburizing gas atmosphere on one side and a decarburizing atmosphere on the other side at 75C. After having reached steady state, the iron was quickly cooled to room temperature. The carbon concentrations at the two surfaces of the sheet were determined to be 0.01 and wt%. Compute the diffusion coefficient if the diffusion flux is kg/m s. Hint: Use Equation 4.9 to convert the concentrations from weight percent to kilograms of carbon per cubic meter of iron. Solution of 5.8: Let us first convert the carbon concentrations from weight percent to kilograms carbon per meter cubed using Equation 4.9a. For 0.01 wt% C C " C C = C C C C 10 3 Fe C Fe = g/cm g/cm Similarly, for wt% C kg C/m 3 C C " = g/cm g/cm Now, using a rearranged form of Equation 5.3 = kg C/m 3 x D = J A x B C A C B = ( kg/m 10 s) 3 m kg/m kg/m 3 = m /s
12 Question 5.11: Determine the carburizing time necessary to achieve a carbon concentration of 0.45 wt% at a position mm into an iron carbon alloy that initially contains 0.0 wt% C. The surface concentration is to be maintained at 1.30 wt% C, and the treatment is to be conducted at 1000C. Use the diffusion data for Fe in Table 5.. Solution of 5.11: In order to solve this problem it is first necessary to use Equation 5.5: C x C 0 x = 1 erf C s C 0 Dt wherein, C x = 0.45, C 0 = 0.0, C s = 1.30, and x = mm = 103 m. Thus, C x C 0 C s C 0 = = 0.73 = 1 erf x Dt or x erf = = Dt By linear interpolation using data from Table 5.1 z erf(z) z z = From which z = = x Dt Now, from Table 5., at 1000C (173 K) D = ( m 148, 000 J/mol /s) exp (8.31 J/mol K)(173 K) Thus, Solving for t yields = m /s = 3 m () ( m /s) (t) t = s = 19.7 h
13 Question 5.1: An FCC ironcarbon alloy initially containing 0.35 wt% C is exposed to an oxygenrich and virtually carbonfree atmosphere at 1400 K (117C). Under these circumstances the carbon diffuses from the alloy and reacts at the surface with the oxygen in the atmosphere; that is, the carbon concentration at the surface position is maintained essentially at 0 wt% C. (This process of carbon depletion is termed decarburization.) At what position will the carbon concentration be 0.15 wt% after a 10h treatment? The value of D at 1400 K is m /s. Solution of 5.1: This problem asks that we determine the position at which the carbon concentration is 0.15 wt% after a 10h heat treatment at 135 K when C 0 = 0.35 wt% C. From Equation 5.5 C x C 0 C s C 0 = Thus, x erf = Dt Using data in Table 5.1 and linear interpolation x = = 1 erf Dt z erf (z) z z = And, Which means that And, finally x Dt z = = x = (0.400) Dt = (0.8004) ( m /s)( s) = m = 1.6 mm Note: this problem may also be solved using the Diffusion module in the VMSE software. Open the Diffusion module, click on the Diffusion Design submodule, and then do the following:
14 1. Enter the given data in lefthand window that appears. In the window below the label D Value enter the value of the diffusion coefficient viz. 6.9e11.. In the window just below the label Initial, C0 enter the initial concentration viz In the window the lies below Surface, Cs enter the surface concentration viz Then in the Diffusion Time t window enter the time in seconds; in 10 h there are (60 s/min)(60 min/h)(10 h) = 36,000 s so enter the value 3.6e4. 5. Next, at the bottom of this window click on the button labeled Add curve. 6. On the right portion of the screen will appear a concentration profile for this particular diffusion situation. A diamondshaped cursor will appear at the upper lefthand corner of the resulting curve. Click and drag this cursor down the curve to the point at which the number below Concentration: reads 0.15 wt%. Then read the value under the Distance:. For this problem, this value (the solution to the problem) is ranges between 1.4 and 1.30 mm.
15 Question 5.15: For a steel alloy it has been determined that a carburizing heat treatment of 10h duration will raise the carbon concentration to 0.45 wt% at a point.5 mm from the surface. Estimate the time necessary to achieve the same concentration at a 5.0mm position for an identical steel and at the same carburizing temperature. Solution of 5.15: This problem calls for an estimate of the time necessary to achieve a carbon concentration of 0.45 wt% at a point 5.0 mm from the surface. From Equation 5.6b, x Dt = constant But since the temperature is constant, so also is D constant, and x = constant t or x 1 = x t 1 t Thus, (.5 mm) 10 h = (5.0 mm) t from which t = 40 h Question 5.16: Cite the values of the diffusion coefficients for the interdiffusion of carbon in both αiron (BCC) and γiron (FCC) at 900 C. Which is larger? Explain why this is the case. Solution 5.16: We are asked to compute the diffusion coefficients of C in both and iron at 900C. Using the data in Table 5., D = ( m 80, 000 J/mol /s) exp (8.31 J/mol K)(1173 K) = m /s D = ( m 148, 000 J/mol /s) exp (8.31 J/mol K)(1173 K) = m /s The D for diffusion of C in BCC iron is larger, the reason being that the atomic packing factor is smaller than for FCC iron (0.68 versus 0.74 Section 3.4); this means that there is slightly more interstitial void space in the BCC Fe, and, therefore, the motion of the interstitial carbon atoms occurs more easily.
16 Question 5.18: At what temperature will the diffusion coefficient for the diffusion of copper in nickel have a value of m /s. Use the diffusion data in Table 5.. Solution of 5.18: Solving for T from Equation 5.9a Q T = d R(ln D ln D 0 ) and using the data from Table 5. for the diffusion of Cu in Ni (i.e., D 0 = m /s and Q d = 56,000 J/mol), we get T = 56,000 J/mol (8.31 J/mol K) ln ( m /s) ln ( m /s) = 115 K = 879C Note: this problem may also be solved using the Diffusion module in the VMSE software. Open the Diffusion module, click on the D vs 1/T Plot submodule, and then do the following: 1. In the lefthand window that appears, there is a preset set of data for several diffusion systems. Click on the box for which Cu is the diffusing species and Ni is the host metal. Next, at the bottom of this window, click the Add Curve button.. A log D versus 1/T plot then appears, with a line for the temperature dependence of the diffusion coefficient for Cu in Ni. At the top of this curve is a diamondshaped cursor. Clickanddrag this cursor down the line to the point at which the entry under the Diff Coeff (D): label reads m /s. The temperature at which the diffusion coefficient has this value is given under the label Temperature (T):. For this problem, the value is 1153 K.
17 Question 5.1: The diffusion coefficients for iron in nickel are given at two temperatures: T (K) D (m /s) (a) Determine the values of D 0 and the activation energy Q d. (b) What is the magnitude of D at 1100ºC (1373 K)? Solution of 5.1: (a) Using Equation 5.9a, we set up two simultaneous equations with Q d and D 0 as unknowns as follows: ln D 1 lnd 0 Q d 1 R T 1 ln D lnd 0 Q d 1 R T Now, solving for Q d in terms of temperatures T 1 and T (173 K and 1473 K) and D 1 and D ( and m /s), we get = (8.31 J/mol K) Q d = R ln D 1 ln D 1 T 1 1 T ln ( ) ln ( ) K K = 5,400 J/mol Now, solving for D 0 from Equation 5.8 (and using the 173 K value of D) D 0 = D 1 exp Q d RT 1 = ( m 5, 400 J/mol /s)exp (8.31 J/mol K)(173 K) = m /s (b) Using these values of D 0 and Q d, D at 1373 K is just D = ( m 5, 400 J/mol /s)exp (8.31 J/mol K)(1373 K) = m /s
18 Note: this problem may also be solved using the Diffusion module in the VMSE software. Open the Diffusion module, click on the D0 and Qd from Experimental Data submodule, and then do the following: 1. In the lefthand window that appears, enter the two temperatures from the table in the book (viz. 173 and 1473, in the first two boxes under the column labeled T (K). Next, enter the corresponding diffusion coefficient values (viz. 9.4e16 and.4e14 ). 3. Next, at the bottom of this window, click the Plot data button. 4. A log D versus 1/T plot then appears, with a line for the temperature dependence for this diffusion system. At the top of this window are give values for D 0 and Q d ; for this specific problem these values are m /s and 5 kj/mol, respectively 5. To solve the (b) part of the problem we utilize the diamondshaped cursor that is located at the top of the line on this plot. Clickanddrag this cursor down the line to the point at which the entry under the Temperature (T): label reads The value of the diffusion coefficient at this temperature is given under the label Diff Coeff (D):. For our problem, this value is m /s.
19 Question 5.4: Carbon is allowed to diffuse through a steel plate 15 mm thick. The concentrations of carbon at the two faces are 0.65 and 0.30 kg C/m 3 Fe, which are maintained constant. If the preexponential and activation energy are m /s and 80,000 J/mol, respectively, compute the temperature at which the diffusion flux is kg/m s. Solution 5.4: Combining Equations 5.3 and 5.8 yields J = D C x C = D 0 x exp Q d RT Solving for T from this expression leads to T = Q d 1 R ln D 0 C J x And incorporation of values provided in the problem statement yields = 80, 000 J/mol J/mol K ln ( m /s)(0.65 kg/m kg/m 3 ) ( kg/m s)( m) = 1044 K = 771C
20 Question 5.30: The outer surface of a steel gear is to be hardened by increasing its carbon content. The carbon is to be supplied from an external carbonrich atmosphere, which is maintained at an elevated temperature. A diffusion heat treatment at 850C (113 K) for 10 min increases the carbon concentration to 0.90 wt% at a position 1.0 mm below the surface. Estimate the diffusion time required at 650C (93 K) to achieve this same concentration also at a 1.0mm position. Assume that the surface carbon content is the same for both heat treatments, which is maintained constant. Use the diffusion data in Table 5. for C diffusion in Fe. Solution of 5.30: In order to compute the diffusion time at 650C to produce a carbon concentration of 0.90 wt% at a position 1.0 mm below the surface we must employ Equation 5.6b with position (x) constant; that is Or Dt = constant D 850 t 850 = D 650 t 650 In addition, it is necessary to compute values for both D 850 and D 650 using Equation 5.8. From Table 5., for the diffusion of C in Fe, Q d = 80,000 J/mol and D 0 = m /s. Therefore, D 850 = ( m 80, 000 J/mol /s)exp (8.31 J/mol K)( K) = m /s D 650 = ( m 80, 000 J/mol /s)exp (8.31 J/mol K)( K) = m /s Now, solving the original equation for t 650 gives t 650 = D 850 t 850 D 650 = ( m /s)(10 min) m /s = 63.9 min
In order to solve this problem it is first necessary to use Equation 5.5: x 2 Dt. = 1 erf. = 1.30, and x = 2 mm = 2 103 m. Thus,
5.3 (a) Compare interstitial and vacancy atomic mechanisms for diffusion. (b) Cite two reasons why interstitial diffusion is normally more rapid than vacancy diffusion. Solution (a) With vacancy diffusion,
More informationThe atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C. = 2(sphere volume) = 2 = V C = 4R
3.5 Show that the atomic packing factor for BCC is 0.68. The atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C Since there are two spheres associated
More informationChapter Outline Dislocations and Strengthening Mechanisms
Chapter Outline Dislocations and Strengthening Mechanisms What is happening in material during plastic deformation? Dislocations and Plastic Deformation Motion of dislocations in response to stress Slip
More informationLösungen Übung Verformung
Lösungen Übung Verformung 1. (a) What is the meaning of T G? (b) To which materials does it apply? (c) What effect does it have on the toughness and on the stress strain diagram? 2. Name the four main
More informationME 612 Metal Forming and Theory of Plasticity. 1. Introduction
Metal Forming and Theory of Plasticity Yrd.Doç. e mail: azsenalp@gyte.edu.tr Makine Mühendisliği Bölümü Gebze Yüksek Teknoloji Enstitüsü In general, it is possible to evaluate metal forming operations
More informationChapter Outline: Phase Transformations in Metals
Chapter Outline: Phase Transformations in Metals Heat Treatment (time and temperature) Microstructure Mechanical Properties Kinetics of phase transformations Multiphase Transformations Phase transformations
More informationIronCarbon Phase Diagram (a review) see Callister Chapter 9
IronCarbon Phase Diagram (a review) see Callister Chapter 9 University of Tennessee, Dept. of Materials Science and Engineering 1 The Iron Iron Carbide (Fe Fe 3 C) Phase Diagram In their simplest form,
More informationModule #17. Work/Strain Hardening. READING LIST DIETER: Ch. 4, pp. 138143; Ch. 6 in Dieter
Module #17 Work/Strain Hardening READING LIST DIETER: Ch. 4, pp. 138143; Ch. 6 in Dieter D. KuhlmannWilsdorf, Trans. AIME, v. 224 (1962) pp. 10471061 Work Hardening RECALL: During plastic deformation,
More informationFundamentals of grain boundaries and grain boundary migration
1. Fundamentals of grain boundaries and grain boundary migration 1.1. Introduction The properties of crystalline metallic materials are determined by their deviation from a perfect crystal lattice, which
More informationWafer Manufacturing. Reading Assignments: Plummer, Chap 3.1~3.4
Wafer Manufacturing Reading Assignments: Plummer, Chap 3.1~3.4 1 Periodic Table Roman letters give valence of the Elements 2 Why Silicon? First transistor, Shockley, Bardeen, Brattain1947 Made by Germanium
More informationx100 A o Percent cold work = %CW = A o A d Yield Stress Work Hardening Why? Cell Structures Pattern Formation
Work Hardening Dislocations interact with each other and assume configurations that restrict the movement of other dislocations. As the dislocation density increases there is an increase in the flow stress
More informationEVERYDAY ENGINEERING EXAMPLES FOR SIMPLE CONCEPTS
EVERYDAY ENGINEERING EXAMPLES FOR SIMPLE CONCEPTS Thermal Properties ENGR 3350  Materials Science Dr. Nedim Vardar Copyright 2015 Thermal Properties of Materials Engage: MSEIP Engineering Everyday Engineering
More informationUnit 12 Practice Test
Name: Class: Date: ID: A Unit 12 Practice Test Multiple Choice Identify the choice that best completes the statement or answers the question. 1) A solid has a very high melting point, great hardness, and
More informationUsing Excel (Microsoft Office 2007 Version) for Graphical Analysis of Data
Using Excel (Microsoft Office 2007 Version) for Graphical Analysis of Data Introduction In several upcoming labs, a primary goal will be to determine the mathematical relationship between two variable
More informationMaterials Issues in Fatigue and Fracture
Materials Issues in Fatigue and Fracture 5.1 Fundamental Concepts 5.2 Ensuring Infinite Life 5.3 Finite Life 5.4 Summary FCP 1 5.1 Fundamental Concepts Structural metals Process of fatigue A simple view
More informationPlate waves in phononic crystals slabs
Acoustics 8 Paris Plate waves in phononic crystals slabs J.J. Chen and B. Bonello CNRS and Paris VI University, INSP  14 rue de Lourmel, 7515 Paris, France chen99nju@gmail.com 41 Acoustics 8 Paris We
More informationEXPERIMENTAL AND NUMERICAL ANALYSIS OF THE COLLAR PRODUCTION ON THE PIERCED FLAT SHEET METAL USING LASER FORMING PROCESS
JOURNAL OF CURRENT RESEARCH IN SCIENCE (ISSN 23225009) CODEN (USA): JCRSDJ 2014, Vol. 2, No. 2, pp:277284 Available at www.jcrs010.com ORIGINAL ARTICLE EXPERIMENTAL AND NUMERICAL ANALYSIS OF THE COLLAR
More information7. 1.00 atm = 760 torr = 760 mm Hg = 101.325 kpa = 14.70 psi. = 0.446 atm. = 0.993 atm. = 107 kpa 760 torr 1 atm 760 mm Hg = 790.
CHATER 3. The atmosphere is a homogeneous mixture (a solution) of gases.. Solids and liquids have essentially fixed volumes and are not able to be compressed easily. have volumes that depend on their conditions,
More informationBending, Forming and Flexing Printed Circuits
Bending, Forming and Flexing Printed Circuits John Coonrod Rogers Corporation Introduction: In the printed circuit board industry there are generally two main types of circuit boards; there are rigid printed
More informationLecture 6 Scanning Tunneling Microscopy (STM) General components of STM; Tunneling current; Feedback system; Tip  the probe.
Lecture 6 Scanning Tunneling Microscopy (STM) General components of STM; Tunneling current; Feedback system; Tip  the probe. Brief Overview of STM Inventors of STM The Nobel Prize in Physics 1986 Nobel
More informationThe entire document shall be read and understood before proceeding with a test. ISTA 3B 2013  Page 1 of 35
PackagedProducts for LessThanTruckload (LTL) Shipment ISTA 3 Series General Simulation Performance Test PROCEDURE VERSION DATE Last TECHNICAL Change: NOVEMBER 2012 Last EDITORIAL Change: JANUARY 2013
More informationXI / PHYSICS FLUIDS IN MOTION 11/PA
Viscosity It is the property of a liquid due to which it flows in the form of layers and each layer opposes the motion of its adjacent layer. Cause of viscosity Consider two neighboring liquid layers A
More informationLesson 3: Isothermal Hydrostatic Spheres. B68: a selfgravitating stable cloud. Hydrostatic selfgravitating spheres. P = "kt 2.
Lesson 3: Isothermal Hydrostatic Spheres B68: a selfgravitating stable cloud Bok Globule Relatively isolated, hence not many external disturbances Though not main mode of star formation, their isolation
More informationQuickstart for Desktop Version
Quickstart for Desktop Version What is GeoGebra? Dynamic Mathematics Software in one easytouse package For learning and teaching at all levels of education Joins interactive 2D and 3D geometry, algebra,
More informationIntegration of a fin experiment into the undergraduate heat transfer laboratory
Integration of a fin experiment into the undergraduate heat transfer laboratory H. I. AbuMulaweh Mechanical Engineering Department, Purdue University at Fort Wayne, Fort Wayne, IN 46805, USA Email: mulaweh@engr.ipfw.edu
More informationManual for simulation of EB processing. Software ModeRTL
1 Manual for simulation of EB processing Software ModeRTL How to get results. Software ModeRTL. Software ModeRTL consists of five thematic modules and service blocks. (See Fig.1). Analytic module is intended
More informationUseful charge on one mole of electrons: 9.64 x 10 4 coulombs/mol e  = F F is the Faraday constant
Electrochemistry II: Cell voltage and Gibbs Free energy Reading: Moore chapter 19, sections 15.615.12 Questions for Review and Thought: 36, 40, 42, 44, 50, 54, 60, 64, 70 Key Concepts and Skills: definition
More informationChapter 1 The Atomic Nature of Matter
Chapter 1 The Atomic Nature of Matter 6. Substances that cannot be decomposed into two or more simpler substances by chemical means are called a. pure substances. b. compounds. c. molecules. d. elements.
More informationT A B L E T 1 T E S T S A N D I N S P E C T I O N C A B L E P C U T A N D P C U T  A
T A B L E T 1 1 of 7 Tests & Inspection Cable PCUT & PCUTA (Table T1) T E S T S A N D I N S P E C T I O N C A B L E P C U T A N D P C U T  A No. Test Scale MOC Requirements G 20:10:001:01 Defined Test
More information= 1.038 atm. 760 mm Hg. = 0.989 atm. d. 767 torr = 767 mm Hg. = 1.01 atm
Chapter 13 Gases 1. Solids and liquids have essentially fixed volumes and are not able to be compressed easily. Gases have volumes that depend on their conditions, and can be compressed or expanded by
More informationXRay Diffraction HOW IT WORKS WHAT IT CAN AND WHAT IT CANNOT TELL US. Hanno zur Loye
XRay Diffraction HOW IT WORKS WHAT IT CAN AND WHAT IT CANNOT TELL US Hanno zur Loye Xrays are electromagnetic radiation of wavelength about 1 Å (1010 m), which is about the same size as an atom. The
More informationModule 1 : Conduction. Lecture 5 : 1D conduction example problems. 2D conduction
Module 1 : Conduction Lecture 5 : 1D conduction example problems. 2D conduction Objectives In this class: An example of optimization for insulation thickness is solved. The 1D conduction is considered
More informationCONCEPT CHECK QUESTIONS AND ANSWERS. Chapter 2 Atomic Structure and Interatomic Bonding
CONCEPT CHECK QUESTIONS AND ANSWERS Chapter 2 Atomic Structure and Interatomic Bonding Concept Check 2.1 Question: Why are the atomic weights of the elements generally not integers? Cite two reasons. Answer:
More informationPrinciples of Electronic Materials and Devices
s Manual to accompany Principles of Electronic Materials and Devices Second Edition S.O. Kasap University of Saskatchewan Boston Burr Ridge, IL Dubuque, IA Madison, WI New York San Francisco St. Louis
More informationXray thinfilm measurement techniques
Technical articles Xray thinfilm measurement techniques II. Outofplane diffraction measurements Toru Mitsunaga* 1. Introduction A thinfilm sample is twodimensionally formed on the surface of a substrate,
More informationModule 34. Heat Treatment of steel IV. Lecture 34. Heat Treatment of steel IV
Module 34 Heat reatment of steel IV Lecture 34 Heat reatment of steel IV 1 Keywords : Austenitization of hypo & hyper eutectoid steel, austenization temperature, effect of heat treatment on structure &
More informationAnalyses on copper samples from Micans
PDF rendering: DokumentID 1473479, Version 1., Status Godkänt, Sekretessklass Öppen Analyses on copper samples from Micans P. Berastegui, M. Hahlin, M. Ottosson, M. Korvela, Y. Andersson, R. Berger and
More informationAdsorption and Catalysis
Adsorption and Catalysis Dr. King Lun Yeung Department of Chemical Engineering Hong Kong University of Science and Technology CENG 511 Lecture 3 Adsorption versus Absorption H H H H H H H H H Adsorption
More informationAnnealing behaviour of plastically deformed stainless steel 1.4307 studied by positron annihilation methods
NUKLEONIKA 2013;58(1):215 219 ORIGINAL PAPER Annealing behaviour of plastically deformed stainless steel 1.4307 studied by positron annihilation methods Ewa Dryzek, Maciej Sarnek, Krzysztof Siemek Abstract.
More informationPOWDER XRAY DIFFRACTION: STRUCTURAL DETERMINATION OF ALKALI HALIDE SALTS
EXPERIMENT 4 POWDER XRAY DIFFRACTION: STRUCTURAL DETERMINATION OF ALKALI HALIDE SALTS I. Introduction The determination of the chemical structure of molecules is indispensable to chemists in their effort
More informationLaser beam sintering of coatings and structures
Laser beam sintering of coatings and structures Anne Maria Reinecke, Peter Regenfuß, Maren Nieher, Sascha Klötzer, Robby Ebert, Horst Exner Laserinstitut Mittelsachsen e.v. an der Hochschule Mittweida,
More informationYSI Meter Protocol: Specific Conductivity, ph, & Dissolved Oxygen
YSI Meter Protocol: Specific Conductivity, ph, & Dissolved Oxygen 1. Check the logbook to see if somebody else has already checked the meter for accuracy within the timeframes below. If the meter hasn
More informationCandidate Style Answer
Candidate Style Answer Chemistry A Unit F321 Atoms, Bonds and Groups High banded response This Support Material booklet is designed to accompany the OCR GCE Chemistry A Specimen Paper F321 for teaching
More informationRAPIDLY SOLIDIFIED COPPER ALLOYS RIBBONS
Association of Metallurgical Engineers of Serbia AMES Scientific paper UDC:669.35153.881412.2=20 RAPIDLY SOLIDIFIED COPPER ALLOYS RIBBONS M. ŠULER 1, L. KOSEC 1, A. C. KNEISSL 2, M. BIZJAK 1, K. RAIĆ
More informationAlloys & Their Phase Diagrams
Alloys & Their Phase Diagrams Objectives of the class Gibbs phase rule Introduction to phase diagram Practice phase diagram Lever rule Important Observation: One question in the midterm Consider the Earth
More informationMathematical Modeling and Engineering Problem Solving
Mathematical Modeling and Engineering Problem Solving Berlin Chen Department of Computer Science & Information Engineering National Taiwan Normal University Reference: 1. Applied Numerical Methods with
More informationABAQUS Tutorial. 3D Modeling
Spring 2011 01/21/11 ABAQUS Tutorial 3D Modeling This exercise intends to demonstrate the steps you would follow in creating and analyzing a simple solid model using ABAQUS CAE. Introduction A solid undergoes
More informationClouds. Ulrike Lohmann Department of Physics and Atmospheric Science, Dalhousie University, Halifax, N. S., Canada
Clouds Ulrike Lohmann Department of Physics and Atmospheric Science, Dalhousie University, Halifax, N. S., Canada Outline of this Lecture Overview of clouds Warm cloud formation Precipitation formation
More informationCorrecting the Lateral Response Artifact in Radiochromic Film Images from Flatbed Scanners
Correcting the Lateral Response Artifact in Radiochromic Film Images from Flatbed Scanners Background The lateral response artifact (LRA) in radiochromic film images from flatbed scanners was first pointed
More informationXray diffraction techniques for thin films
Xray diffraction techniques for thin films Rigaku Corporation Application Laboratory Takayuki Konya 1 Today s contents (PM) Introduction Xray diffraction method OutofPlane InPlane Pole figure Reciprocal
More informationCarbon Cable. Sergio Rubio Carles Paul Albert Monte
Carbon Cable Sergio Rubio Carles Paul Albert Monte Carbon, Copper and Manganine PhYsical PropERTieS CARBON PROPERTIES Carbon physical Properties Temperature Coefficient α 0,0005 ºC1 Density D 2260 kg/m3
More informationThe ratio of inertial to viscous forces is commonly used to scale fluid flow, and is called the Reynolds number, given as:
12.001 LAB 3C: STOKES FLOW DUE: WEDNESDAY, MARCH 9 Lab Overview and Background The viscosity of a fluid describes its resistance to deformation. Water has a very low viscosity; the force of gravity causes
More informationRelease notes: ThermoCalc software package 4.1
Release notes: ThermoCalc software package 4.1 19952014 Foundation of Computational Thermodynamics Stockholm, Sweden Introduction Contents Release notes This document provides information on new products,
More informationElectrochemistry Revised 04/29/15
INTRODUCTION TO ELECTROCHEMISTRY: CURRENT, VOLTAGE, BATTERIES, & THE NERNST EQUATION Experiment partially adapted from J. Chem. Educ., 2008, 85 (8), p 1116 Introduction Electrochemical cell In this experiment,
More information2 Absorbing Solar Energy
2 Absorbing Solar Energy 2.1 Air Mass and the Solar Spectrum Now that we have introduced the solar cell, it is time to introduce the source of the energy the sun. The sun has many properties that could
More information1.1 DIMENSIONS AND WEIGHT PAG. 2 1.2 LOAD CENTRE FOR LIFTING PAG. 2 1.3 STORAGE CONDITIONS PAG. 2
TRANSPORT AND INSTALLATION. DIMENSIONS AND WEIGHT PAG.. LOAD CENTRE FOR LIFTING PAG..3 STORAGE CONDITIONS PAG. STARTING. INSTALLATION PAG.. SPACE REQUIREMENTS PAG. 3.3 ELECTRIC CONNECTION PAG. 3 3 DESCRIPTION
More information10 g 5 g? 10 g 5 g. 10 g 5 g. scale
The International System of Units, or the SI Units Vs. Honors Chem 1 LENGTH In the SI, the base unit of length is the Meter. Prefixes identify additional units of length, based on the meter. Smaller than
More informationDetermining the Quantity of Iron in a Vitamin Tablet. Evaluation copy
Determining the Quantity of Iron in a Vitamin Tablet Computer 34 As biochemical research becomes more sophisticated, we are learning more about the role of metallic elements in the human body. For example,
More informationChapter 22: Electric Flux and Gauss s Law
22.1 ntroduction We have seen in chapter 21 that determining the electric field of a continuous charge distribution can become very complicated for some charge distributions. t would be desirable if we
More informationMODEL 9020 & 9020OEM CORRATER TRANSMITTER USER MANUAL
Serial Number MODEL 9020 & 9020OEM CORRATER TRANSMITTER USER MANUAL ROHRBACK COSASCO SYSTEMS, INC. 11841 East Smith Avenue Santa Fe Springs, CA 90670 Tel: (562) 9490123 (800) 6356898 Fax: (562) 9493065
More informationTHE CONCEPT OF VISCOSITY
CHAPTER 3 THE CONCEPT OF VISCOSITY Fluid flow plays a very important part in the processing of materials. Most processes are based on the use of fluids either as raw materials, reagents, or heat transfer
More informationFigure 10.1. Process flow from starting material to polished wafer.
Figure 10.1. Process flow from starting material to polished wafer. 1/11/003 Ettore Vittone Fisica dei Semiconduttori  Lectio XI 1 Starting material: silicon dioxide (SiO ): pure form of sand (quartzite)
More informationChapter 3, Lesson 4: Density: Sink and Float for Solids
Chapter 3, Lesson 4: Density: Sink and Float for Solids Key Concepts The density of an object determines whether it will float or sink in another substance. An object will float if it is less dense than
More informationAP Physics 1 and 2 Lab Investigations
AP Physics 1 and 2 Lab Investigations Student Guide to Data Analysis New York, NY. College Board, Advanced Placement, Advanced Placement Program, AP, AP Central, and the acorn logo are registered trademarks
More informationDislocation Plasticity: Overview
Dislocation Plasticity: Overview 1. DISLOCATIONS AND PLASTIC DEFORMATION An arbitrary deformation of a material can always be described as the sum of a change in volume and a change in shape at constant
More informationSpaceClaim Introduction Training Session. A SpaceClaim Support Document
SpaceClaim Introduction Training Session A SpaceClaim Support Document In this class we will walk through the basic tools used to create and modify models in SpaceClaim. Introduction We will focus on:
More informationChemical Kinetics. Reaction Rate: The change in the concentration of a reactant or a product with time (M/s). Reactant Products A B
Reaction Rates: Chemical Kinetics Reaction Rate: The change in the concentration of a reactant or a product with time (M/s). Reactant Products A B change in number of moles of B Average rate = change in
More informationL 2 : x = s + 1, y = s, z = 4s + 4. 3. Suppose that C has coordinates (x, y, z). Then from the vector equality AC = BD, one has
The line L through the points A and B is parallel to the vector AB = 3, 2, and has parametric equations x = 3t + 2, y = 2t +, z = t Therefore, the intersection point of the line with the plane should satisfy:
More informationNatural Convection. Buoyancy force
Natural Convection In natural convection, the fluid motion occurs by natural means such as buoyancy. Since the fluid velocity associated with natural convection is relatively low, the heat transfer coefficient
More informationBINARY SYSTEMS. Definition of Composition: Atomic (molar) fraction. Atomic percent. Mass fraction. Mass percent (weight percent)
BINARY SYSTEMS Definition of Composition: Atomic (molar) fraction Atomic percent Mass fraction Mass percent (weight percent) na =, x i n = A i i i Weight percent mainly in industry! x at % A = x 100 A
More informationGeoGebra. 10 lessons. Gerrit Stols
GeoGebra in 10 lessons Gerrit Stols Acknowledgements GeoGebra is dynamic mathematics open source (free) software for learning and teaching mathematics in schools. It was developed by Markus Hohenwarter
More information(1) e.g. H hydrogen that has lost 1 electron c. anion  negatively charged atoms that gain electrons 162. (1) e.g. HCO 3 bicarbonate anion
GS106 Chemical Bonds and Chemistry of Water c:wou:gs106:sp2002:chem.wpd I. Introduction A. Hierarchy of chemical substances 1. atoms of elements  smallest particles of matter with unique physical and
More informationChapter 13  Solutions
= Chapter 13  Solutions Description: Find the weight of a cylindrical iron rod given its area and length and the density of iron. Part A On a parttime job you are asked to bring a cylindrical iron rod
More informationh e l p s y o u C O N T R O L
contamination analysis for compound semiconductors ANALYTICAL SERVICES B u r i e d d e f e c t s, E v a n s A n a l y t i c a l g r o u p h e l p s y o u C O N T R O L C O N T A M I N A T I O N Contamination
More informationAn introduction to 3D draughting & solid modelling using AutoCAD
An introduction to 3D draughting & solid modelling using AutoCAD Faculty of Technology University of Plymouth Drake Circus Plymouth PL4 8AA These notes are to be used in conjunction with the AutoCAD software
More informationDiffusion and Fluid Flow
Diffusion and Fluid Flow What determines the diffusion coefficient? What determines fluid flow? 1. Diffusion: Diffusion refers to the transport of substance against a concentration gradient. ΔS>0 Mass
More informationFigure 1. A voltaic cell Cu,Cu 2+ Ag +, Ag. gas is, by convention, assigned a reduction potential of 0.00 V.
Voltaic Cells Introduction In this lab you will first prepare a set of simple standard halfcells and then measure the voltage between the halfcells with a voltmeter. From this data you will be able to
More informationMicroscopy and Nanoindentation. Combining Orientation Imaging. to investigate localized. deformation behaviour. Felix Reinauer
Combining Orientation Imaging Microscopy and Nanoindentation to investigate localized deformation behaviour Felix Reinauer René de Kloe Matt Nowell Introduction Anisotropy in crystalline materials Presentation
More informationA reinterpretation of the phase transitions in Na 2 CO 3
Acta Crystallographica Section B Structural Science ISSN 01087681 Editor: Carolyn P. Brock A reinterpretation of the phase transitions in Na 2 CO 3 Alla Arakcheeva and Gervais Chapuis Copyright International
More informationRoHSCompliant ThroughHole VI Chip Soldering Recommendations
APPLICATION NOTE AN:017 RoHSCompliant ThroughHole VI Chip Soldering Recommendations Ankur Patel Associate Product Line Engineer Contents Page Introduction 1 Wave Soldering 1 Hand Soldering 4 Pin/Lead
More informationIntroduction to Autodesk Inventor for F1 in Schools
Introduction to Autodesk Inventor for F1 in Schools F1 in Schools Race Car In this course you will be introduced to Autodesk Inventor, which is the centerpiece of Autodesk s digital prototyping strategy
More informationSUS. Company Profile. Ulrich Nell, Feldstr.23, D  46149 Oberhausen, Tel. 0049(0)208/658535 Fax 0049(0)208/658536
SUS Ulrich Nell, Feldstr.23, D  46149 Oberhausen, Tel. 0049(0208/658535 Fax 0049(0208/658536 Company Profile SUS was founded in 1986 in Oberhausen in the Ruhr area (close to Düsseldorf, in order to meet
More informationPractice Tests Answer Keys
Practice Tests Answer Keys COURSE OUTLINE: Module # Name Practice Test included Module 1: Basic Math Refresher Module 2: Fractions, Decimals and Percents Module 3: Measurement Conversions Module 4: Linear,
More informationMillikan Oil Drop. Introduction
Millikan Oil Drop Introduction Towards the end of the 19th century a clear picture of the atom was only beginning to emerge. An important aspect of this developing picture was the microscopic nature of
More informationThe OPERA Emulsions. Jan Lenkeit. Hamburg Student Seminar, 12 June 2008. Institut für Experimentalphysik Forschungsgruppe Neutrinophysik
The OPERA Emulsions Jan Lenkeit Institut für Experimentalphysik Forschungsgruppe Neutrinophysik Hamburg Student Seminar, 12 June 2008 1/43 Outline The OPERA experiment Nuclear emulsions The OPERA emulsions
More informationProject 1.3.4 Renewable Insulation Example Teacher Notes
Project 1.3.4 Renewable Insulation Example Teacher Notes Sample Data and Teacher Notes This guide is designed to provide sample calculations, background, and tips for the teachers performing this project
More informationInvestigation of Titanium α Plates by EBSD Analysis
Investigation of Titanium α Plates by EBSD Analysis Master Thesis Arjen Kamp June 2007 Materials Science and Engineering Faculty 3mE Supervisors: Stefan van Bohemen Jilt Sietsma Roumen Petrov Investigation
More informationMicrosoft Mathematics for Educators:
Microsoft Mathematics for Educators: Familiarize yourself with the interface When you first open Microsoft Mathematics, you ll see the following elements displayed: 1. The Calculator Pad which includes
More informationTABLE OF CONTENTS. INTRODUCTION... 5 Advance Concrete... 5 Where to find information?... 6 INSTALLATION... 7 STARTING ADVANCE CONCRETE...
Starting Guide TABLE OF CONTENTS INTRODUCTION... 5 Advance Concrete... 5 Where to find information?... 6 INSTALLATION... 7 STARTING ADVANCE CONCRETE... 7 ADVANCE CONCRETE USER INTERFACE... 7 Other important
More informationThermokinetics based materials modeling with MatCalc Functionality and integration
http://matcalc.at Thermokinetics based materials modeling with MatCalc Functionality and integration E. Kozeschnik Outline General information Thermodynamic engine Equilibrium and nonequilibrium thermodynamics
More informationDrawing a histogram using Excel
Drawing a histogram using Excel STEP 1: Examine the data to decide how many class intervals you need and what the class boundaries should be. (In an assignment you may be told what class boundaries to
More informationPrinted Circuit Board Recycling Methods
Printed Circuit Board Recycling Methods 1. Introduction to Printed Circuit Boards The Printed Circuit Board (PCB 1 ) manufacturing process is very complicated, involving many special chemicals and valuable
More informationPaper No. 4071 APPLICATION OF EQCM TO THE STUDY OF CO2 CORROSION
Paper No. 471 APPLICATION OF EQCM TO THE STUDY OF CO2 CORROSION Yang Yang, Bruce Brown and Srdjan Nešić Institute for Corrosion and Multiphase Technology, Department of Chemical and Biomolecular Engineering
More informationBonds. Bond Length. Forces that hold groups of atoms together and make them function as a unit. Bond Energy. Chapter 8. Bonding: General Concepts
Bonds hapter 8 Bonding: General oncepts Forces that hold groups of atoms together and make them function as a unit. Bond Energy Bond Length It is the energy required to break a bond. The distance where
More informationFREESTUDY HEAT TRANSFER TUTORIAL 3 ADVANCED STUDIES
FREESTUDY HEAT TRANSFER TUTORIAL ADVANCED STUDIES This is the third tutorial in the series on heat transfer and covers some of the advanced theory of convection. The tutorials are designed to bring the
More informationState Newton's second law of motion for a particle, defining carefully each term used.
5 Question 1. [Marks 28] An unmarked police car P is, travelling at the legal speed limit, v P, on a straight section of highway. At time t = 0, the police car is overtaken by a car C, which is speeding
More informationHeat transfer efficiency improvement in highpressure metal hydride by modeling approach
International Journal of Smart Grid and Clean Energy Heat transfer efficiency improvement in highpressure metal hydride by modeling approach Nur Aisyah Jalalludin a*, Noboru Katayama b, Sumio Kogoshi
More informationPrussian blue nanoparticles for laserinduced photothermal therapy of tumors
Electronic Supplementary Material (ESI) for RSC Advances. This journal is The Royal Society of Chemistry 2014 Supporting Information Prussian blue nanoparticles for laserinduced photothermal therapy of
More informationHeterogeneous Catalysis and Catalytic Processes Prof. K. K. Pant Department of Chemical Engineering Indian Institute of Technology, Delhi
Heterogeneous Catalysis and Catalytic Processes Prof. K. K. Pant Department of Chemical Engineering Indian Institute of Technology, Delhi Module  03 Lecture 10 Good morning. In my last lecture, I was
More information9781467319652/12/$31.00 2012 IEEE 1488
Generic Thermal Analysis for Phone and Tablet Systems Siva P. Gurrum, Darvin R. Edwards, Thomas MarchandGolder, Jotaro Akiyama, Satoshi Yokoya, JeanFrancois Drouard, Franck Dahan Texas Instruments, Inc.,
More information